SHAHRIN, RAHNUMA. Nanoindentation Investigation of FIB-Milled Microstructures to Assess Failure Properties of Cement Paste at Microscale. (Under the direction of Dr. Christopher Bobko and Dr. Mohammad Pour-Ghaz).
A mechanical test methodology using Focused Ion Beam (FIB) milled micropillars and nanoindentation is developed to investigate the failure mechanism of cement paste at the level of calcium-silicate-hydrates (C-S-H), the primary binding phase of concrete. Cement paste is a hierarchical material with different levels spanning the range from nanometers to hundreds of micrometers. C-S-H is primarily responsible for strength and other mechanical properties of cement based materials. Therefore, a fundamental understanding and quantification of the failure behavior of C-S-H at microscale is critical for understanding failure at larger scales. Current experimental techniques, however, are unable to reveal how compressive failure is initiated within the cement paste microstructure. Therefore, a need exists for the development of a robust experimental method that can characterize compressive strength and failure modes of C-S-H.
Nanoindentation Investigation of FIB-Milled Microstructures to Assess Failure Properties of Cement Paste at Microscale
A dissertation submitted to the Graduate Faculty of North Carolina State University
in partial fulfillment of the requirements for the degree of
Doctor of Philosophy
Raleigh, North Carolina 2018
Dr. Christopher Bobko, Dr. Mohammad Pour-Ghaz,
Committee Co-Chair Committee Co-Chair
Rahnuma Shahrin was born in Chittagong, Bangladesh and spent her childhood in four different cities of Bangladesh. She earned her B.Sc. in Civil Engineering from Bangladesh University of Engineering and Technology (BUET) in 2009 and graduated first in her class. After graduation, she joined the same university as a faculty of Structural Engineering and did teaching and research for four years. In 2013, she completed her M.Sc. in Civil
(Structural) engineering from Bangladesh University of Engineering and Technology
I would like to express my sincere respect and gratitude to my primary advisor, Dr.
Christopher Bobko for being a knowledgeable, enthusiastic and extremely supportive mentor. I am greatly indebted to him for shaping my critical-thinking and academic writing
perspectives. His continuous motivation and guidance encouraged me to explore the unknown and become the independent researcher and scientist that I am today.
I am also grateful to Dr. Mohammad Pour-Ghaz for his thoughtful insight, guidance, logistic support and continuous encouragement throughout my PhD journey. I would also like to thank Dr. Murthy Guddati and Dr. Chih-Hao Chang for their feedbacks, suggestions and continued guidance. My sincere gratitude to head of the CCEE department, Dr. Morton Barlaz and director of graduate program, Dr. Ranji Ranjithan for their strong support throughout my program.
I want to thank my husband Shams, for his endless love, support and sacrifices. Thank you for always believing in my capabilities. Thanks to my parents and sisters for their
unconditional love and my friends at Raleigh for always being there.
TABLE OF CONTENTS
List of Tables ……….………...ix
List of Figures ………..…….xi
Chapter 1: Introduction 1.1 General ………... 1
1.2 Research Needs ………2
1.3 Research Tasks ………3
1.4 Outline ……….. 3
Chapter 2: Literature Review 2.1 Introduction ………....5
2.2 Motivation for Nanoscale Experiments ………....5
2.2.1 Multiscale overview of concrete ………6
2.2.2 Nano scale properties of C-S-H ………8
2.3 Overview of Nanoindentation Investigations on Cementitious Material …………9
2.4 Effect of Water/Cement Ratio ………..12
2.5 SEM Investigations on Cementitious Material ………..13
2.5.1 Use of BSE imaging ………..13
2.5.2 Use of EDS microanalysis ………..14
2.5.3 Use of FIB sectioning ………..15
2.6 Limitations of Strength Measurement in Cement ………..16
2.7 Coupled FIB-milling/NI- testing Approach for Strength Measurement ………..18
2.7.1 Developing micro-structures using fib milling ………..18
2.7.2 Estimation of compressive strength ………..22
2.7.3 Estimation of elastic modulus ………..24
2.7.4 Investigation of size effect ………..25
Chapter 3: Materials and Methods
3.1 Introduction ………..29
3.2 Materials ………..29
3.2.1 Cement ………..29
3.2.2 Belite ………..30
3.3 Sample preparation ………..31
3.3.1 Surface preparation ………..31
3.3.2 Coating ………..33
3.4 Fabrication of Micropillars: ……….…….33
3.4.1 Introduction to the instrument ………..…34
3.4.2 Determining location of micropillar milling ………..36
3.4.3 Selection of size ………..43
3.4.4 Annular milling method ………..45
3.5 Micro-Compression Testing ………..48
3.5.1 Equipment and calibration: ………..48
3.5.2 Loading protocol: ………..50
3.5.3 Use of micrograph ………..55
3.6 Post-test Imaging ………..57
3.7 Estimation of Strength ………..58
3.8 Estimation of Elastic Modulus ………..61
3.9 Size Effect Analysis ………..64
3.10 Summary ………..65
Chapter 4: Assessment of Strength and Failure Modes 4.1 Introduction ………..66
4.2 Microstructure of Stochiometric Cement Paste ………..66
4.2.2 Microstructure Observations from coupled FIB milling and SE imaging ..67
4.3 Failure Modes ………..69
4.3.1 Axial splitting ………..70
4.3.2 Shearing ………..71
4.3.3 Crushing ………..72
4.3.4 Combination mode ………..73
4.3.5 Unknown mode ………..73
4.3.6 Failure due to local irregularity ………..74
4.4 Load-Displacement Behavior and Strength ………..75
4.5 Effect of Ca/Si ratio ………..81
4.6 Discussion ………..82
4.7 Summary ………..84
Chapter 5: Effect of Sample Size 5.1 Introduction ………..86
5.2 Experimental Program ………..………86
5.3 Stress-Strain behavior ………..……88
5.4 Size-Effect for Strength ………..………98
5.5 Size-Effect for Modulus ………102
5.6 Comparison of Failure Modes ………103
5.7 Discussions ………107
5.7.1 Effect of Weak link on Strength and Deformation Mode………..…………107
5.7.2 Modeling Perspective ………108
5.7.3 Estimation of Fracture Toughness from Observed Failure Behavior ...……110
5.8 Summary ………112
6.2 Experimental Program ………113
6.3 Strength and Modulus Results ………116
6.4 Comparison of Strength Results for Different w/c ratios and Different Phases……119
6.5 Comparison of Failure Modes ………121
6.6 Summary ………125
Chapter 7: Conclusions 7.1 Summary and Key Findings ………127
7.2 Future Work ………129
LIST OF TABLES
Table 2.1 FIB milling conditions used by some other investigators for fabrication
of micropillars (Shim et al. 2009) ...21
Table 3.1 Bogue Composition of a typical Type I/II Portland cement ...30
Table 3.2 Calculation of Ca/Si ratio from area under the peak ...43
Table 3.3 Details of tested micropillar samples and materials ...45
Table 3.4 List of parameters used in FIB milling of cement micropillars ...48
Table 3.5 Parameter list for single cycle tests...52
Table 3.6 Parameter List for Multi cycle tests on 0.42 w/c ratio cement ...54
Table 3.7 Optimized parameters for post-test imaging using Verios SEM ...58
Table 3.8 Loading and unloading moduli measured for stress-strain plot in Figure 3.28 ...64
Table 4.1 Dimension, mechanical, and chemical properties of the tested w/c= 0.42 micropillars. Here (𝐷𝐷1) and (𝐷𝐷2) are top and bottom diameters, (𝐻𝐻) is the height, and (𝐻𝐻⁄ ((((𝐷𝐷1) + (𝐷𝐷2))⁄2) )) is the aspect ratio of micropillars. (𝐶𝐶𝐶𝐶/𝑆𝑆𝑆𝑆) is the calcium to silicon ratio of the micropillar location. ...80
Table 4.2 Average compressive strength for the three primary failure modes ...81
Table 5.1 No of final sample of each size considered for size effect analysis ...88
Table 5.2 Dimension, mechanical and chemical properties of the smaller diameter micropillars. Here (𝐷𝐷1) and (𝐷𝐷2) are top and bottom diameters, (𝐻𝐻) is the height, and (𝐻𝐻) ⁄ ((((𝐷𝐷1)) + (𝐷𝐷2)))⁄2) )) is the aspect ratio of micropillars. (𝐶𝐶𝐶𝐶/𝑆𝑆𝑆𝑆) is the calcium to silicon ratio of the micropillar location. ...98
Table 5.3 Comparison of average failure stress ...99
x Table 6.1 Compressive strength and elastic modulus results for 0.35 and 0.30 w/c ratio sample ...118 Table 6.2 Average compressive strength for each w/c ratio sample ...121 Table 6.3 Percentage of different failure modes observed in different w/c ratio
LIST OF FIGURES
Figure 2.1 Multiscale model of concrete (Constantinides and Ulm 2007b), Level 0
drawing from (Allen et al. 2007), level I image from (Nonat 2004) ...7 Figure 2.2 Formation of C-S-H gel a) One relatively small volume fractal region of
C-S-H globules. b) Same volume fractal region (shown in white) has grown into a larger, self-similar structure with a reduced packing density.
c) Adjacent fractal regions have grown (Jennings et al. 2007) ...9 Figure 2.3 Volume fraction distribution of hydrated phases in cement paste with
different w/c (Vandamme and Ulm 2009) ...13 Figure 2.4 Concentric rings and trench formed by annular milling on a) metallic glass (Yang et al. 2009) b) Ni single crystal (Uchic and Dimiduk 2005) ...19 Figure 2.5 (a) Schematic of uniaxial compression on micropillar (b) A representative stress-strain curve (Han et al. 2011) ...23 Figure 2.6 Size effect observed in yield stress for gold (Au) micropillars (Volkert
and Lilleodden 2006) ...26 Figure 2.7 Size effect in uniaxial compression of concrete cylinders (Yi et al. 2006a) ...27 Figure 3.1 Disk shaped and cylindrical cement samples of a) 0.42 b) 0.35 and c) 0.30 water to cement ratio ...30 Figure 3.2 Disk shaped belite paste sample after removing from mold ...31 Figure 3.3 a) Large scale saw, and b) Buehler Isomet low speed saw used for cutting cement sample ...32 Figure 3.4 Saw cut thin cement sample on polisher machine ...32 Figure 3.5 Optical microscope micrograph of a 0.42 w/c ratio cement sample after
45 min polishing a) 100X objective view b) 20X objective view ...33 Figure 3.6 Sputter coated cement slice in SEM stub ...33 Figure 3.7 Representative SEM image showing series of micropillars milled on a
0.42 w/c ratio cement sample surface. The scratch marks around are allow easy identification of the location in optical microscope...34 Figure 3.8 a) Focused Ion Beam (FIB) SEM b) schematic diagram explaining
xii Figure 3.10 Signal generation depth for different type of SEM techniques.
Secondary electrons (SE) are detected from close to the surface, backscatter electrons (BSE) from a somewhat greater depth and characteristic X-rays are generated throughout the interaction
(Scrivener 2004)...37 Figure 3.11 Typical BSE image of a) w/c = 0.42 and b) w/c =0.3 cement pastes with the individual microscopic phases distinguished by contrast ...39 Figure 3.12 a) BSE image of a w/c = 0.35 cement paste showing formation of HD
CSH rim around partially reacted clinker b) two micropillars fabricated in dark grey areas close to clinker grains. ...40 Figure 3.13 The interaction volume probed by SEM/EDS is approximated by Monte Carlo simulation as the zone demarcated by the electron trajectories (blue lines) in the specimen...41 Figure 3.14 Location of EDS analysis selected in grey region for spectrum shown below in Figure 3.15 ...42 Figure 3.15 A representative EDS spectrum collected on a C-S-H location
(Ca/Si =1.87) ...43 Figure 3.16 Representative SEM image of a micropillar explaining the dimension
terms ...45 Figure 3.17 Annular milling of micropillar shown in five steps: from milling of
outer ring to fabrication of final pillar geometry ...47 Figure 3.18 Representative SEM image of FIB-milled micropillars showing
dimension measured from high magnification image ...48 Figure 3.19 a) Schematic of CSM Instruments Ultra Nano Hardness Tester
(UNHT) construction b) Test set-up c) Schematic of indenter tip geometry ..50 Figure 3.20 Schematic of uniaxial compression on the micropillar ...51 Figure 3.21 Representative a) Load-time and b) load-displacement plot of a
monotonic single cycle micro-compression test showing sudden load
drop and displacement jump ...53 Figure 3.22 Load-time plot showing trapezoidal loading segments with linearly
xiii (b) higher magnification image showing top view of a 2-µm diameter
micropillar inside a 25-µm diameter trench ...57 Figure 3.24 Field Emission Scanning Electron Microscope (SEM) used for performing post-test image analysis ...58 Figure 3.25 a) Load and displacement plotted against time b) Load versus
displacement plot; sudden load drop and displacement jump is observed at failure, only few data points are collected in the failure zone ...60 Figure 3.26 Measurement of failure load in multi-cycle test from load-displacement plot ...61 Figure 3.27 a) Stress-strain behavior up to failure b) Measurement of loading elastic modulus from linear portion of stress-strain plot ...62 Figure 3.28 Representative stress-strain behavior at multi-cycle test...63 Figure 4.1 Backscattered electron image of hydrated cement paste showing different phases present in a stochiometric (w/c = 0.42) paste ...67 Figure 4.2 SE image of FIB milled region showing boundary of distinct phases ...68 Figure 4.3 Distinguishable features of micropillars milled on a-b) LD C-S-H c-d) HD C-S-H and e) clinker ...69 Figure 4.4 a-c) Micropillars showing various type of axial splitting d) side wall
cracking failure ...71 Figure 4.5 Micropillars showing shearing failure with formation of diagonal crack ...72 Figure 4.6 Micropillars showing plastic crushing failure with signs of damage on top ...73 Figure 4.7 Micropillars showing both plastic crushing and cracking (combined)
mode of failure ...73 Figure 4.8 Micropillar geometries with unknown mode of failure ...74 Figure 4.9 Micropillars failed due to local irregularity; a) porous bottom
b-c) uneven milling of sidewalls ...75 Figure 4.10 Representative load-displacement curves for types of failure modes-
a) axial splitting b) side wall cracking c) shearing d) crushing
xiv a) 2 µm b) 1.5 µm c) 1 µm and d) 0.5 µm ...87 Figure 5.2 Load-displacement curve for micro-compression of a) 1.5µm b) 1 µm and c) 0.5 µm diameter pillars ...89 Figure 5.3 Stress-strain curves up to failure (marked by x) for micro-compression
of a) 1.5µm b) 1 µm and c) 0.5 µm diameter pillars. 4 curves of each size are shown for clarity of image ...94 Figure 5.4 Displacement-time plot for a 1.5 µm diameter pillar (yellow one in
Figure 6.3a) showing variation of displacement increase during constant peak loads...97 Figure 5.5 Compressive strength of micropillars plotted against top diameter.
Compressive strength shows an overall increase with decrease in pillar diameter. The solid line indicates best fitted a) linear and
b) power relationship. ...101 Figure 5.6 Elastic (Young’s) modulus of micropillars plotted against top diameter. ...102 Figure 5.7 Appearance of 1.5 µm diameter pillars after failure by a) axial splitting b) crushing and c) shearing ...104 Figure 5.8 Appearance of 1 µm diameter pillars after failure by a) crushing and
b) shearing c) axial splitting and d) side splitting ...105 Figure 5.9 Appearance of 0.5 µm diameter pillars after failure by a) shearing
b) crushing of top c) and crushing of entire pillar. Most of the pillars
of 0.5 diameter showed crushing of entire pillar like c...106 Figure 5.10 SEM images showing failure due to presence of weak link in the
micropillar. a-b) micro-cracks c-d) porosity e-f) transition zone ...109 Figure 5.11 Presence of a pre-existing crack (large pore) of ~ 500 nm. ...112 Figure 6.1 BSE images showing difference of microstructure in a) 0.42 w/c ratio
b) 0.35 w/c ratio and c) 0.30 w/c ratio paste ...115 Figure 6.2 Representative image of micropillars on a) w/c 0.42 b) w/c 0.35 and
c) w/c 0.30 sample ...116 Figure 6.3 Relationship between strength and elastic modulus for a) w/c 0.35
xv d) crushing (top), and e) localized failure at interphase failure modes
observed for w/c 0.35 sample ...123 Figure 6.6 a) Axial splitting b) splitting sample with interacting microcracks
c) shearing d) crushing (top) and e) local failure at top failure modes
Concrete is the single most widely used material in the world. From tower blocks to carparks – this material is used so widely in construction industry that production, transportation, and use of concrete accounts for between 5-9% of total CO2 emissions worldwide (Metz 2005).
Cement paste is the binder and key ingredient of concrete, and a hierarchical material itself with three different levels spanning the range from few nanometers to hundreds of micrometers (Constantinides and Ulm 2004). It is composed of an amorphous phase calcium-silicate-hydrate (C–S–H) that acts as a matrix and binds the inclusions of Ca(OH)2, unhydrated cement
clinkers, water and micrometer range of porosity to form cement paste (Hlobil et al. 2015). C– S–H is the glue that holds concrete together and is itself a nanomaterial. Having different properties at each length scale (from nano to macro), the properties of concrete at each scale derives from those of the next smaller scale. There is a strong evidence that the processes occurring at the small scale ultimately affect the engineering properties and performance of the bulk material. Therefore, if the fundamental mechanisms behind failure of cement can be better understood at small scale, rationally designed engineering solutions can be deployed to provide tougher materials for civil infrastructure, reducing consumption of natural resources and production of CO2. In this context, the primary research objectives of this work are to measure
2 and Ulm 2004; Constantinides and Ulm 2007; Vandamme and Ulm 2009). However, investigation of failure properties of cement at this length scale is not that straightforward and hence gained less focus in nanoindentation literature.
In recent years, material scientists have introduced small-scale compression tests of micro-pillars using a customized nanoindentation system (Uchic et al. 2003). For preparing specimens suitable for such small-scale experiments, the focused ion beam (FIB) techniques are employed. Since then uniaxial compression of focused ion beam (FIB) milled micropillars using nanoindentation equipment has become an effective approach to investigate small scale strength properties (Uchic et al. 2004; Ye et al. 2010; Volkert and Lilleodden 2006; Shim et al. 2009; Korte and Clegg 2009). FIB based micro-compression tests attained greater interest and attention for various kinds of materials such as – bulk metallic glasses, shape memory alloys and single crystals. Yet, few studies have explored the application of micro-compression testing to granular and heterogeneous materials such as bones, mudstones, shales, and dental enamel- which have hierarchical microstructure like cement paste (Zhang et al. 2010; Abousleiman et al. 2016; Yilmaz et al. 2015; An et al. 2015; Dewers et al. 2010; Han et al. 2011; Luczynski et al. 2015). While one study has used FIB milled microbeams to assess tensile strength of cement (Němeček et al. 2016), uniaxial compression tests have never been performed on FIB milled cement micropillars for assessing their compressive failure behavior. In this thesis a new methodology is developed to provide a quantitative portrait of failure behavior cement paste at level-1. This study is one of the first to explore how FIB based micro-compression techniques can be applied to improve our understanding of failure of cementitious materials.
1.2 Research Needs
The following research needs and potential scope for making contributions are identified in the subsequent literature review section:
a. Current experimental research cannot reveal how failure is generated within cement paste microstructure.
3 c. The deformation mechanism of C-S-H phases under compressive failure load is yet to
d. Innovative sample preparation techniques are required for making micron sized sample geometries on individual phases of cement.
1.3 Research Tasks
In accordance to the needs established in literature review and the gaps mentioned in section 1.1, the following tasks will help to achieve the research objective:
a. To develop a repeatable sample preparation method for creating cement paste micro-pillars using FIB milling.
b. To establish a robust experimental protocol for testing the FIB-milled sample geometries in uniaxial compression using nanoindentation system.
c. To obtain a data set of compressive strength and elastic modulus of C-S-H phase by analysis of raw data from micro-compression tests.
d. To determine the effect of w/c ratio and pillar size on compressive strength, elastic modulus, and deformation modes at failure.
e. To link the mechanical responses from experimental observations to different C-S-H packings.
The organization of this thesis consists of seven chapters.
4 system is discussed next. After that, data analysis method for assessing strength and elastic modulus results and post-test SEM imaging techniques for assessing deformation modes is discussed. Finally, specific details related to size effect analysis study is provided.
Chapter 4: This chapter investigates compressive failure behaviors of C-S-H by presenting results of micro-compression experiments on cement micropillars of a constant water to cement ratio and fixed micropillar size. Characterization of C-S-H microstructure, compressive strength and failure modes is performed by analysis of micro-compression results in terms of stress and strain as well as visual observations.
Chapter 5: This chapter focuses on investigating size effect on compressive failure of C-S-H by presenting results of micro-compression experiments on C-S-H micropillars of diameters varying between 2.5 and 0.5 µm fabricated on a constant w/c ratio cement paste. A discussion of the results is presented in the context of existing size-effect models for strength of quasi-brittle materials.
Chapter 6: Effect of cement paste composition on the failure behavior is examined in this chapter by presenting results of micro-compression experiments on C-S-H micropillars from cement pastes with varying w/c ratio. An approach considering elastic modulus obtained in the micro-compression experiments, in conjunction with prior research using grid nanoindentation, is used to propose a range of compressive strengths for cement hydration projects.
2 LITERATURE REVIEW
In this section, a brief description is provided on the multiscale nature of concrete and its main binding phase C-S-H (Section 2.2). The mechanism, capabilities and limitations of existing nanoindentation techniques are reviewed in Section 2.3. Previous investigations on cementitious materials using various features of scanning electron microscopy (SEM) are listed in Section 2.5. Limited available literature on micro-scale measurement of cement strength is discussed in Section 2.6. The potential of FIB based micro-compression experiments in measuring strength properties is discussed in Section 2.7 using related literature. The effect of water to cement ratio on mechanical properties of C-S-H is described in Section 2.4.
2.2 Motivation for Nanoscale Experiments
Concrete is a particularly complex material because it is highly heterogeneous with multiple length scales involved. It is primarily composed of cement paste, sand, coarse aggregate and admixtures in some cases. Each of these ingredients are heterogeneous themselves at a certain level of observation and have different strength and stiffness. Therefore, the heterogeneity of concrete exists in a variety of length scales from nano to macro. It is widely recognized that many macroscopic phenomena of concrete originate from the mechanics of the underlying nano and microscale structure. All the mechanical, physical and chemical properties of the ingredients including strength, stiffness, size, shape, volume fraction, and spatial distribution can have impact on the material behavior observed at macroscale. However, measurements made at the typical scales of concrete laboratory testing are unable to reveal how failure is initiated within the microstructure of cement paste. Small scale experimental techniques are required to quantitatively assess the complex material behaviors that lead to failure in cement paste microstructure. A fundamental understanding of the failure behavior at small scale would result in better prediction and control on the macroscopic concrete properties.
2.2.1 Multiscale overview of concrete
The range of the random microstructure of concrete encompasses nine orders of magnitude in size from nanometer (10-9m) to meters (m). Experimental methods and analytical approaches to understand strength properties of cement and concrete must respect the different material behaviors that are associated with each length scale. Figure 2.1 shows a multi-scale model framework for concrete.
Macroscopic concrete is a three phase material composed of aggregates embedded in a mortar matrix and an ITZ. Fine aggregate (sand), cement paste, entrained air bubbles in cement paste, and crushed coarse aggregates are constituents that make up the mortar. The importance of the aggregate-cement paste interfacial zone, as the third and weakest component of concrete, has been recognized for some time (Monteiro 2006; Monteiro and Mehta 1985). Together, these three phases characterize the macroscopic performance of concrete. Due to large dimension of the composite at this level, mechanical features can be obtained by standard test methods such as compressive cylinder tests
Calcium-Silicate-Hydrates (C-S-H)1 matrix together with large Calcium Hydroxide (CH) crystals, unhydrated cement clinker, ettringite and micrometer porosity in the case of high w/c ratios, forms the cement paste, and is referred to as Level II. Scanning electron microscope (SEM) has good resolutions at this scale, and can be used to observe morphology detail of hydration products with large crystals such as CH and ettringite. Components in this level are also visible in a high-powered optical microscope but with much less resolution and depth of field compared to SEM.
Level I is the smallest material length scale that is, at present, accessible by mechanical testing. A granular composite of C-S-H aggregates and pore space comprise this face which is also called C-S-H gel. At this scale, different C-S-H packing densities, and small capillary pores greater than 10 nm characterize the behavior of the matrix (Jennings et al. 2007). According to the model proposed by Jennings, C-S-H nanoparticles are packed in two different packing densities so called Low density (LD) and High density (HD) C-S-H. The average pore volume
1 In Cement chemistry, C=CaO, S=SiO
2, H=H2O. The atomic elements without oxides are expressed in a
7 of these C-S-H phases were reported 37% and 24% respectively (Jennings 2000). For low w/c ratio pastes Vandamme and colleagues identified the presence of a third type of C-S-H with higher indentation modulus and indentation hardness (Vandamme and Ulm 2009; Vandamme et al. 2010). This phase is termed either as ultra-high density (UHD) C-S-H or C-S-H/CH nanocomposite in different literature (Vandamme and Ulm 2009; Chen et al. 2010).
At Level 0, C-S-H have complicated, non-regular molecular structures. These molecules tend to organize themselves into grains which are termed as C-S-H globules. Using observations from Small Angle Neutron Scattering (SANS), Jennings (Jennings et al. 2007) termed this globules with characteristic size of 5.6 nm as the elementary block of C-S-H aggregates. Richardson used transmission electron micrographs to analyze their morphology and nano structure (Richardson 2004). He classified C-S-H aggregates as inner and outer product of hydration based on their fine-scale like and foil like morphology respectively.
Figure 2.1: Multiscale model of concrete (Constantinides and Ulm 2007b), Level 0 drawing from (Allen et al. 2007), level I image from (Nonat 2004).
Quasi-brittle failure likely initiates at the scale of Level I because at Level 0, mechanical properties within individual C-S-H globules are dominated by strength of chemical bonds.
Level II Cement Paste
C-S-H globules Macroscopic Concrete
8 Failure instead begins within aggregates of C-S-H, which are viewed as granular systems of C-S-H globules.
2.2.2 Nano scale properties of C-S-H
Calcium silicate hydrate (C-S-H) is a highly disordered nano-scale material comprised of layers of calcium and oxygen, with SiO2tetrahedra attached and interspersed by water and
further Ca ions. It is formed in a dissolution-precipitation reaction involving mixtures of tricalcium silicate (Alite) and dicalcium silicate (Belite) with water. Due to the importance of C-S-H as the binder phase of Portland cement it has been widely studied over many decades.
Yet, the link between composition, nano and microstructure and mechanical behavior of C–S– H remains a complex puzzle that is not resolved completely.
Grudemo (Grudemo 1955) was one of the first to propose that the C-S-H gel comprised “solid” regions of layers including some ‘chemically combined’ water with small water filled pores between these regions now widely known as gel pores. From a compositional point of view, the C-S-H gels are often characterised by their Ca/Si ratio, which is in the range from 0.7 to 2.3. The reasons behind this variation might be since C-S-H structure formed by cement hydration is highly dependent on the chemical mixtures and reaction conditions and may evolve over long periods of time.
Density results of different studies and calculations have been reviewed by Jenningsin the context of the colloidal model and vary between 1.8 and 2.8 g/cm3 (Jennings 2008). Much of
this variability arises from the fraction of the gel pore water and other nanoscale confined or bound water that is, or is not, inferred to be included in the measurement. A widely cited result used small angle neutron scattering (SANS) and reported the density for solid crystalline C-S-H to be 2.604 g/cm3 (Allen et al. 2007). In a comparatively recent work, nuclear magnetic resonance (NMR) was used to measure C-S-H density. Depending upon the degree of hydration the reported values for solid density vary in the range of 2.73 ~ 2.65 g/cm3 (Muller
et al. 2012).
The morphology of C-S-H continued to be the subject of active debate in the literature. From atomic force microscope (AFM) investigations Nonat, suggested a brick-type morphology of the C-S-H nanoparticle (lamellae) of dimension 60 x30 x 5nm3 (Nonat 2004). Richardson
9 for the inner product and two distinct morphologies for outer product, a fibrillar structure and a foil-like structure that appear to correlate with the Ca/Siratio (Richardson 2004). The foil-like structure preferentially forms below a Ca/Si ratio of about 1.5. Constantinides and Ulm identified packing density as the key factor behind two distinct C-S-H morphologies, so called, low and high density (Constantinides and Ulm 2004a). Jennigs and coworkers proposed a colloidal model of C-S-H based on results from various experimental techniques (Jennings et al. 2007). According to this model (Figure 2.2) around 5 nm sized globules of C-S-H pack together to form larger structures with lower densities, and in mature pastes there are distinct “high-density” (HD) and “low-density” (LD) morphologies of C-S-H gel depending on packing density. In a different approach, Pellenq and coworkers used bottom-up atomistic simulation to propose a molecular model of C-S-H. This model provides molecular description of interacting CaO, SiO2, and H2O unit and suggests that the C-S-H gel structure includes both
glass-like short-range order and crystalline features of the mineral tobermorite (Pellenq et al. 2009).
Figure 2.2: Formation of C-S-H gel a) One relatively small volume fractal region of C-S-H globules. b) Same volume fractal region (shown in white) has grown into a larger, self-similar structure with a reduced packing density. c) Adjacent fractal regions have grown (Jennings et al. 2007).
2.3 Overview of Nanoindentation Investigations on Cementitious Material
While there have been a variety of available techniques for measuring physical properties and observing the microstructure, experimental investigation of mechanical properties at such
10 small scale is not that straightforward. In last few decades, instrumented indentation, also known as depth sensing indentation or nanoindentation has become a versatile tool to probe the mechanical response of materials from metals polymers, and ceramics to biological materials. Advances in hardware and software control currently enable accurate measurements of the continuous variation of indentation load down to micro Newtons, as a function of the indentation depth down to nanometers. Thus, instrumented indentation provides a convenient, non-destructive means to evaluate the basic mechanical response of small material volumes. The commercially available packages, with flexibility of choosing the appropriate geometry of the indenter tip, have made it an effective way of material characterization for bulk, thin film, or composite materials.
In comparison to homogenous materials, nanoindentation on heterogeneous materials have some added challenges, as it is difficult to choose to indent on a specific material phase with sufficient repeatability. To overcome this difficulty for heterogeneous materials like cement paste, researchers prefer the grid indentation technique coupled with statistical methods. In such cases, the grid size and depth of indentation are the two key parameters that need careful consideration (Ulm et al. 2007).
The initial instrumented indentation efforts reported on cementitious materials were microindentation tests. Igarashi et al. used a Vickers indenter to assess bulk properties of cement paste at a sub-millimeter to millimeter material length scale (Igarashi et al. 1996). Zhu et al. studied the mechanical properties of interfacial transition zone for reinforced concrete (Zhu and Bartos 1997; Zhu and Bartos 2000). Kholmyansky et al. discussed possible experimental methods for determination of hardness in case of fine grained concrete (Kholmyansky et al. 1994). Continuous evolution of computer technology enabled improved control over instrumented indentation testing. In two individual studies, Velez and Acker reported the initial attempts of performing nanoindentation testing on cement (Velez et al. 2001; Acker 2001). Velez studied the elastic modulus and the hardness of the major phases of Portland cements (C3S and alite, C2S and belite, C3A, C4AF) (Velez et al. 2001). Acker
investigated ultra-high performance cementitious composite material, DUCTAL, and reported modulus and hardness values for portlandite (Ca(OH)2) and the C-S-H gel with different Ca/Si
11 Over the last decade, researchers extensively used nanoindentation as a versatile tool to investigate different mechanical properties of cement and concrete. A major portion of this research is centered on determining elastic modulus and hardness values. Constantinides and Ulm investigated the modulus and hardness values for portlandite and C-S-H gel. They used the indentation results as a basis to propose the existence of low and high density C-S-H (Constantinides and Ulm 2004b). Mondal and Shah reported individual modulus and hardness results for low, high and middle density C-S-H by using an in-situ scanning probe microscopy imaging technique of nanoindenter (Mondal et al. 2007). Zhu and his group used progressive multistep indentation tests results and interpolation to develop 2D contour maps of modulus and hardness values for cement paste (Zhu et al. 2007). Trtik and his group determined modulus and hardness results for different individual phases, with primary focus on linking physical observations of microstructure to mechanical responses (Trtik et al. 2009; Hughes and Trtik 2004). They also emphasized the importance of good surface preparation and flat topography for reduced scatter in indentation results. Detail study on surface roughness criteria for cement paste nanoindentation was performed by Miller and coworkers (Miller et al. 2008). They explained a stepwise process as well as the importance of low surface roughness to ensure repeatable and meaningful nanoindentation results.
12 Many nanoindentation studies analyzed creep properties of C-S-H. Vandamme and Ulm used cement pastes of different compositions and water cement ratios to conclude that the logarithmic creep of C–S–H is due to nano-particle sliding within C-S-H that leads to a local increase of the packing density (Vandamme and Ulm 2009). In a subsequent work, they extended their work for several loading protocols and indenter geometry and quantified the amplitude of logarithmic creep by a contact creep modulus. In another concurrent study, Pichler and Lackner used nanaoindentation results for Identification of creep-compliance parameters for logarithmic creep behaviour of of C-S-H (Pichler and Lackner 2009). Němeček discussed the effect of creep deformation while determining the elastic properties of hydrated cement paste. He suggested application of long dwelling time in conjunction with cyclic loading for avoiding creep effects in elastic property measurements (Němeček 2009).
2.4 Effect of Water/Cement Ratio
Figure 2.3: Volume fraction distribution of hydrated phases in cement paste with different w/c (Vandamme and Ulm 2009).
2.5 SEM Investigations on Cementitious Material
Scanning electron microscope (SEM) has been a powerful tool for analysis of cementitious materials for several decades. For cement clinker and hydration products, it permits observation of microstructure and identification of phases, including qualitative as well as quantitative analysis of chemical compositions. The advantage of electron microscopy is all the components of the cement microstructure can be examined at a wide range of magnifications which provides information about their spatial distribution.
2.5.1 Use of BSE imaging
Backscattered electrons are electrons from the incident beam which are reflected or scattered back from the specimen by elastic scattering interactions with specimen atoms. The contrast in BSE signal is produced by the difference is atomic number among the different constituent phases of a sample. The initial users of SEM mostly utilized backscattered electron (BSE) imaging of polished cement sections to distinguish anhydrous material, calcium hydroxide, C-S-H and porosity based on their grey level intensity (Kjellsen et al. 1990; Scrivener et al. 1986). Famy and coworkers used grey level variations to further distinguish between C-S-H gels formed at different temperatures (Famy et al. 2002b). With the advancement of digital
0.03 0.30 0.47 0.50 0.03 0.74 0.52 0.35 0.29 0.97
0.23 0.18 0.18 0.21
0.00 0.20 0.40 0.60 0.80 1.00
0.15 0.20 0.30 0.35 0.40
14 image analysis, quantitative potential of BSE imaging was discovered. BSE imaging was shown to have significant potential of estimating the pore size distribution in concrete (Diamond 2000). Other contemporary works focused diverse applications like mass fraction estimation of the main phases in Portland cement clinker, estimation of water/cement ratio in hardened cement paste and calculation of volume fractions in the interfacial transition zone (Stutzman 2004; Sahu et al. 2004; Scrivener 2004; Campbell 1999). Some researchers used X-ray powder diffraction (XRD) and Rietveld analysis along with backscattered electron for determining amounts of different phases in anhydrous cementitious materials (Scrivener 2004; Stutzman and Leigh 2007). However, BSE imaging is still mostly used qualitatively for identification of different material phases in cementitious materials.
2.5.2 Use of EDS microanalysis
For compositional microanalysis, energy-dispersive spectroscopy (EDS), which is also known as energy-dispersive X-Ray (EDX) is an alternate approach that provides detailed information on chemistry of constituent phases. In contrast to the 2D surface information gathered through BSE imaging, X-Ray microanalysis represents a 3D interaction volume from which the X-Ray is generated. Many researchers have investigated cement pastes by using X-Ray microanalysis. Harrison and coworkers were one of the pioneers who examined the compositions of residual clinker phases by using X-Ray (Harrisson et al. 1986). Richardson and Groves used electron microprobe analysis (EMPA) to get composition for inner and outer product of C-S-H (Richardson and Groves 1993). They used cut off ratio for Ca/Si and (Al + Fe)/Ca and presence of Magnesium to distinguish this two type of C-S-H. Following a similar approach, Bonen and Diamond also analyzed cement paste and reported the present of another C-S-H phase with slightly different composition. They attributed intermixing of Ca(OH)2 with C-S-H gel below
15 but very similar indentation responses at submicron scale is the advantage of such chemo-mechanical analysis. Based on Monte-Carlo simulation, Chen and coworkers argued that the microvolumes probed by SEM-EDS and nanoindentation are directly comparable (Chen et al. 2010). They performed EDS analysis on each of the indentation point and used the composition data to group the indentation results for different phases. Based on the Ca/Si ratio, this work reinforced the presence of a C-S-H /CH nanocomposite. In a similar methodology, indentation response of the C-S-H solid was linked to its stoichiometry via x-ray microanalysis (Krakowiak et al. 2013). In recent years, couple of researchers have used this technique to investigate hydrated phases of cement paste, specifically, C-S-H and CSH/CH nanocomposites (Bu et al. 2015; Moser et al. 2013). This coupled approach provided a promising way to study the local mechanical properties of cement paste and of its constituents by correlating them to their chemical composition.
2.5.3 Use of FIB sectioning
16 used the FIB-nt datasets with improved image processing technique to further distinguish between different phases of hydration products (Trtik et al. 2011).
Some of the researchers used the previously discussed approach of combing indentation results with microstructural investigations for FIB sectioning instead of EDS (Trtik et al. 2009; Lura et al. 2011). By utilizing the nano scale resolution of the ion column, FIB techniques permitted observation of deformed material underneath the indents and hence better understanding of processes which occur during micro or nanoindentation tests. Trtik and his group reported carrying out microindentation experiments on a cementious composite followed by FIB cross sectioning at selected indent points (Trtik et al. 2000; Bartos 2004). SEM micrographs collected from FIB milled trenches were used to gather information about the possible failure modes induced by the impression of diamond indenter in the surrounding material.
2.6 Limitations of Strength Measurement in Cement
Broadly, the SEM investigations literature is centered around identification of main constituent phases in cement, their pore size distribution, chemical composition, and analysis of cement microstructure and morphology. the majority of nanoindentation literature, On the other hand, focuses on measurement of Young’s modulus and hardness values of cement paste constituents. For Von-mises type of materials, a rule-of-thumb relation between (Eq. 2.1) indentation hardness (𝐻𝐻) and tensile strength (𝜎𝜎𝑌𝑌) of the material exists (Tabor 1948)
𝐻𝐻= 3𝜎𝜎𝑌𝑌 (2.1)
Based on this classical relation, the indentation hardness of the metals is often used as an indicator of the strength properties. However, for cohesive materials, very different set of elastic moduli, work hardening exponent and yield strength can result in similar indentation hardness results. Hence, for granular and cohesive materials like cement paste with more complicated strength behaviors, a single indentation hardness measurement cannot be related to strength (Chen et al. 2007).
17 loaded the cubes with a sharp indenter to measure splitting tensile strength, elastic modulus and fracture mechanisms of cement paste at global level (Šavija et al. 2017; Zhang et al. 2017; Zhang et al. 2016). It is important to note that, theses measured properties, due to the large size of the cubes and beams, are representative of the entire paste and not of individual constituent phases,
The strength properties and failure modes of cement paste at the Level I scale has not yet been well investigated. Hlobil et al. estimated compressive strength of C-S-H matrix at Level I using coupled finite element simulations and multiscale analysis for upscaling to practical measures (Hlobil et al. 2016; Hlobil et al. 2015). This approach, however, calculates tensile strength of C-S-H globules based on their approximate packing density and used them as input parameter for compressive behavior of C-S-H matrix, which imposes intrinsic limitations on its predictions.
At Level 0, molecular dynamics simulations provided some insight about the material behavior within the C-S-H globules (Pellenq et al. 2009; Selvam et al. 2009). Yet, the complex granular microstructure of C-S-H aggregates at Level I presents a system far too large for feasible atomistic computations.
In the framework of continuum micromechanics, Pichler and Hellmich and Pichler et al. calculated deviatoric strength of microscopic hydrates based on an elasto-brittle multiscale model for cementitious materials (Pichler and Hellmich 2011; Pichler et al. 2013). The corresponding model predicted uniaxial compressive strength of low-density C-S-H using parameters from finite-element reanalysis of nanoindentation results (Pichler et al. 2013; Sarris and Constantinides 2013). However, the representative volume element (RVE) considered in this model (~20 µm) for strength homogenization, is too large compared to size of individual hydrated phases observed in BSE imaging of hydrated cement paste (Famy et al. 2002a). Moreover, the input parameters used for homogenization, are not properties specific to LD C-S-H, but rather calculated as an average over all type of hydrates, including ettringite, portlandite, and C-S-H of different mass densities.
18 density C-S-H, portlandite, or unhydrated clinker phases. Hence, there is a need for a robust experimental technique that can be used to obtain quantitative information about compressive failure behavior at Level I.
2.7 Coupled FIB-milling/NI- testing Approach for Strength Measurement
For strength measurement of individual phases present at the scale of Level I, it is crucial to develop localized micro-structured sample geometries on the targeted individual components of hydrated cement paste. To achieve this, an effective sample preparation technique is required that can isolate individual phases without disrupting their intrinsic properties.
A recent innovative technique in material science involves testing of FIB milled microstructures (micropillars, micro-beams and wedges) using a nanoindentation tip for measurement of strength (compressive and tensile), fracture toughness and deformation modes. Different micro-machined sample geometries can deliver different material properties, just like their more traditionally sized counterparts. Though nanoindentation systems are designed for performing depth sensing indentation experiments using sharp indenter, when outfitted with a flat or spherical indentation tip, the same platform can be used to perform conventional uniaxial compression tests at prescribed load or displacement rates (Uchic et al. 2004a; Uchic et al. 2003). uniaxial compression testing of FIB milled micro-pillars as unconfined cylinders using nanoindentation equipment provide plastic strength properties of the tested material. The flat tip of the indenter and the attachment of the micropillar to the bulk material functions as the compression platen. In recent years, this micro-compression technique has been extensively used to investigate small scale compressive strength, failure mechanisms, elastic modulus and size effect.
2.7.1 Developing micro-structures using FIB milling
19 the rate at which material is removed remains same throughout the sample surface. Therefore, development of micropillars and more complex geometries like single and double cantilever beams on homogenous materials is reported in various literature (Liu et al. 2013; Riedl et al. 2012; Schaufler et al. 2012).
Different milling methods has been practiced for fabricating micropillars. The ‘ion-lathe method’ is effective but more time intensive (Uchic et al. 2004a; Uchic et al. 2003; Uchic and Dimiduk 2005). Since instrumentation time is critical issue, as an alternative approach, sequential milling of concentric rings also known as ‘annular milling method’ is widely used by researchers (Figure 2.4a). This method allows the user to change milling parameters before each milling cycle. While preparing samples for subsequent micro compression test, formation of a trench like crater has been recommend by many studies (Volkert and Lilleodden 2006; Volkert et al. 2008). Particular advantages of this trenching (Figure 2.4b) lies in (i) allowing one to image the sidewalls of the micro-sample both before and after deformation using the SEM (which is necessary for subsequent fabrication steps), (ii) avoiding the possibility of unintended contact between the indenter tip and the micro-sample, (iii) reducing the probability that sputtered material will redeposit back onto the freshly milled microsample during subsequent fabrication steps, and (iv) facilitating easy identification of the testing location with optical microscope of the nanoindenter test system during testing (Uchic and Dimiduk 2005).
Figure 2.4: Concentric rings and trench formed by annular milling on a) metallic glass ((Yang et al. 2009) b) Ni single crystal (Uchic and Dimiduk 2005).
20 Proper selection of milling parameters plays the key role in successful fabrication of pillar geometry. However, very few studies publish the used parameters. A brief list of the parameters used by some researchers is provided in Table 2.1. As seen from this table, most of the researchers reported using the same acceleration voltage of 30 keV, whereas, the beam current values show a wide variation. Using beam currents as high as 7 nA or higher can significantly reduce the milling time. However, excessive high currents have increased potential of introducing various damage in the micropillar structure (Shim et al. 2009; Thompson et al. 2007). Among all the possible defects, implantation of Gallium ions within the milled material possess the biggest concern in case of amorphous materials. Such implantations have the potential to affect small scale mechanical behavior. According to Thompson et al., use of lower beam currents can reduce this damage to a significant extent (Thompson et al. 2007).
Table 2.1: FIB milling conditions used by some other investigators for fabrication of micropillars (Shim et al. 2009).
Authors Materials FIB milling conditions
Uchic et al. Single-crystal Ni and Ni3Al Not reported
Single-crystal superalloy Accelerating voltage: 30 keV Beam current: 1–7 nA for coarse milling, and 0.05–1 nA for fine milling
Single-crystal Ni Not reported Pure Ni and Ni3Al Not reported Greer et al. Single-crystal Au Not reported Single-crystal Au and Mo Not reported
Volkert et al. Single-crystal Au Accelerating voltage: 30 keV Beam current: not reported Kiener et al. Single-crystal Cu Accelerating voltage: 30 keV
Beam current: 1 nA for coarse milling, and 0.1 nA for fine milling
Shan et al. Single-crystal Ni Not reported
Ng et al. Polycrystal Al Accelerating voltage: not
reported Beam current: 20 nA for coarse milling, and 0.05 nA for fine milling
Frick et al. Single-crystal Ni Not reported Norfleet et al. Single-crystal Ni Not reported
22 like cementitious materials (Dewers et al. 2010; Han et al. 2011; Yilmaz et al. 2015; Yilmaz et al. 2013; Yilmaz et al. 2013; Zhang et al. 2010; An et al. 2015). Researchers explored the application of micro-compression and micro-bending testing of FIB-milled structures for heterogeneous shale material which exhibit hierarchical microstructure like cement paste. Abousleiman et al. tested FIB milled cantilever micro-beams in bending using nanoindenter tip, and studied tensile strength characteristics of shale (Abousleiman et al. 2016). Keller et al applied micropillar compression testing to measure Microscale uniaxial compressive strength and stiffness of shale (Keller et al. ). Very recently, FIB milling has been performed on cement for fabrication of microbeams for measurement of tensile strength (Němeček et al. 2016; Chen et al. 2015). However, FIB milled micropillars geometries have never been reported to be fabricated on cement.
2.7.2 Estimation of compressive strength
Figure 2.5: (a) Schematic of uniaxial compression on micropillar (b) A representative stress-strain curve (Han et al. 2011).
A closed loop trapezoidal compression loading needs to be imposed on micro-compression samples by controlling either the loading or the displacement. In both cases, a holding time of 5-15 second is preferred between the loading and unloading to remove creep effect. Uchic et al. followed the displacement controlled approach with a displacement rate of 1-5 nm/s (Uchic and Dimiduk 2005). Han et al. also used a similar approach with 5 nm/s loading rate and a prescribed maximum displacement of 120 nm (Han et al. 2011). Alternatively, the force can be controlled with a prescribed loading rate (Volkert and Lilleodden 2006; Volkert et al. 2008; Shim et al. 2009). However, it is important to note that most nanoindentation systems use voice coils as the force actuator, thus the instrument inherently become a load-controlled test system.
The extraction of stress-strain behavior from the load-displacement curve requires estimation of the pillar dimensions. Due to the increased complexities in measuring pillar dimensions after test, engineering stress and strains are used instead of true stress (Han et al. 2011). Estimation of the effective cross-sectional area needs to be done depending on the type of deformation that is observed at failure. Considering the taper in pillar sidewalls, some researchers have used average of top and bottom diameter of the pillar or the mid height diameter for estimation of effective cross- sectional area (Volkert and Lilleodden 2006). For materials that exhibit highly localized deformation, pillar dimensions should be measured in the region where the deformation typically occurs (Shim et al. 2009). For pillars that are formed on a substrate material having different properties, combined effect of the compression of the micropillar and
24 the indentation of the pillar into the underlying bulk material can be accounted for by applying Sneddon’s formula (Sneddon 1965). Considering the substrate compliance, the normalized engineering stress 𝜎𝜎𝑛𝑛 and strain 𝜀𝜀𝑛𝑛 for the slightly tapered pillars were calculated by Han et al. as using loading portions of the force (𝐹𝐹) versus compression depth (𝛿𝛿) curves
𝜀𝜀𝑛𝑛 = 𝐻𝐻𝛿𝛿 (2.2)
𝜎𝜎𝑛𝑛 =�𝜋𝜋𝐷𝐷4 1𝐷𝐷2 +
1− 𝜈𝜈2 𝐷𝐷2𝐻𝐻 � 𝐹𝐹
Here, 𝜈𝜈 is approximated Poisson’s ratio of substrate, 𝐻𝐻 is the pillar height, and 𝐷𝐷1 and 𝐷𝐷2 are the diameters of the top and bottom face of the pillar. The elastic modulus,𝐸𝐸, is extracted from the elastic portion of the normalized stress versus strain curve via least-squares linear regression (Han et al. 2011).
Han et al. considered the first point where the load dropped below 95% of the force predicted by slope of the elastic portion. Denoting that load by𝐹𝐹𝑌𝑌 (Figure 2.5b), the strength is estimated as,
𝜎𝜎𝑌𝑌 = 𝜋𝜋𝐷𝐷4𝐹𝐹𝑌𝑌 12
2.7.3 Estimation of elastic modulus
25 which they attributed to the lack of proper contact between the sample and tip and resulting stress localization during initial loading of the samples (Uchic and Dimiduk 2005).
Simulation of micro-compression studies suggested that lack of perfect contact between indenter tip and pillar is more pronounced at lower compression depths which reduces the elastic modulus of the loading curve. Nonetheless, better contact is achieved with increasing compression depth, and the unloading curve is not affected by this experimental issue. Hence, many researchers have performed multi-cycle loading-unloading micro-compression tests and used unloading moduli for measurement of elastic modulus.(Yilmaz et al. 2015; Frick et al. 2008; Camposilvan and Anglada 2016; Greer et al. 2005). Some researchers calculated elastic modulus from a linear fit to the initial 20% of unloading curve (Yilmaz et al. 2015; Choi et al. 2012). Yilmaz et al (2015) observed gradual increase in elastic modulus from the unloading slopes of successive loading cycles, for multi-cycle tests on dental enamel micropillars. They attributed this increase in modulus to improve contact between pillar and indenter at larger compression depths and reported the elastic modulus value from the penultimate cycle as the final elastic modulus.
2.7.4 Investigation of size effect
The size effect is understood as dependence of the structure strength on the structure size. In recent literature, micro-compression experiments on crystalline and amorphous metals have shown the presence of size effect on both strength and elastic modulus. The ease of varying the deformation length-scale and the availability of high resolution load–displacement data makes FIB-based micro-compression well suited for studying size effects in materials. For Ni-based single crystals, Uchic et al. reported a strong dependence of yield strength on inverse of the square root of pillar diameter by testing pillars ranging in the size range of 0.5 to 40 µm in diameter (Uchic et al. 2003; Uchic et al. 2004b). Volkert and Lilleodden showed strong increase in yield strength (𝜎𝜎𝑌𝑌)of Au as pillar diameter (𝑑𝑑) decreases from 8 µm to 180 nm gradually (Volkert and Lilleodden 2006). They proposed a best fit to the yield stress data (Figure 2.6) as
Figure 2.6: Size effect observed in yield stress for gold (Au) micropillars (Volkert and Lilleodden 2006).
Ye et al. also mentioned the size dependent deformation behavior of micropillars and normalized the yield strength results using the elastic modulus (Ye et al. 2010). Yang et al. reported another form of size dependence which is observed in case of Young’s modulus. Their work showed a spurious dependence of micropillar’s Young’s modulus on its aspect ratio (Yang et al. 2009b). It is also observed that the deformation mechanism that leads to compressive failure is also dependent on the pillar size (Volkert et al. 2008).
For the prediction of size effect in concrete, Bazant derived the size effect law (SEL) for geometrically similar structures of different sizes with initial crack using the energy balance approach of linear elastic fracture mechanics (LEFM) (Bazant and Planas 1997). The equation has the basic form
𝜎𝜎𝑁𝑁𝑁𝑁 = 𝐵𝐵𝑓𝑓𝑡𝑡 ′
�1 + 𝐷𝐷𝐷𝐷
27 For quasi-brittle compression failure of concrete columns, Bazant suggested an asymptotic size effect law where the size effect coefficient can be expressed by power law 𝐷𝐷−2/5 for larger sizes of cross-section (Bažant and Xiang 1997). In this asymptotic size effect law, the size effect asymptotically disappears towards a limiting small size of cross section.
For concrete cylinders, researchers have reported effect of cylinder size on compressive strength of plain concrete cylinders (Kim et al. 1999; Yi et al. 2006)(Figure 2.7). Kim et al. derived the following size effect equation (Eq. 2.7)
𝑓𝑓0 = 0.8 𝑓𝑓𝑐𝑐′+ 0.4 𝑓𝑓𝑐𝑐 ′
�1 + (ℎ − 𝑑𝑑)/50 (2.7)
for cylindrical concrete specimen subjected to uniaxial compression loads based on Bazant’s size effect law.
Figure 2.7: Size effect in uniaxial compression of concrete cylinders (Yi et al. 2006).
28 2.8 Summary
Literature reviews were mainly focused on four major areas: motivation behind small-scale experiments on cement, various SEM investigation methods for cementitious materials, capabilities and limitation of conventional nanoindentation techniques, and potential use of FIB based micro-compression studies in investigating failure mechanisms.
Major findings from this section are –
• Heterogeneity of concrete exists in a variety of length scales. To understand failure properties of concrete and cement, experimental methods must respect the differential material behavior associated with each length scale.
• Principal binding phase of cement, C-S-H, is a granular composite with varying packing densities. Previous SEM and nanoindentation studies confirmed the presence of distinct low (LD), high density (HD) and ultra-high-density C-S-H phases.
• Water to cement ratio (w/c) influences the relative volume fractions of low (LD), high density (HD) and ultra-high-density C-S-H phases in cement paste. However, their elastic modulus values are independent of mixing proportions.
• Existing nanoindentation techniques are capable of measuring volume fractions and mechanical properties such as elastic modulus, hardness and creep parameters for C-S-H. Nanoindentation results can be coupled with EDS analysis for correlating mechanical responses to distinct chemical phases. However, compressive strength cannot be measured using conventional nanoindentation techniques.
• Recent approach of uniaxial compression testing of micropillar using customized nanoindentation system provides strength measurements at micrometer and sub micrometer scale.
• FIB milling method of preparing micropillar geometries is commonly used for homogenous materials. However, successful application of this method for heterogeneous and granular materials is reported in recent studies.
3 Materials and Methods
This chapter describes the methodological approach of this research, specifically developed and modified for application to cementitious materials. First, an introduction to the cementitious materials studied in this research is provided with details of their preliminary surface preparation techniques. Then, the method of micropillar fabrication using focused ion beam (FIB) milling is described in detail. Next, methodology of uniaxial compression testing of FIB milled micropillars using nanoindentation system is described. After that, analysis of indentation results for assessing individual strength and elastic modulus results and post-test SEM investigation of deformed pillars for assessing deformation modes is discussed. Finally, specific details related to size effect analysis study is provided.
Sample materials were carefully chosen to be representative of the basic form of cement paste. Regular type I/II cement with a water/cement (w/c) ratio of 0.42 was selected as the primary test material. The typical composition of a type I/II cement is shown in Table 3.1. According to Powers’ hydration model, w/c of 0.42 is considered adequate for complete and unimpeded hydration. No admixtures or supplementary cementitious materials were added to this paste. The cement paste was cured under sealed condition to achieve full hydration and development of strength for three years. Specimens were cut in disk shape (Figure 3.1) and again stored in airtight containers to avoid change of mechanical properties until they were used in the FIB sample preparation process. For studying the effect of sub-stochiometric conditions (w/c< 0.42) on measured mechanical properties, two samples were prepared with less amount of water (w/c 0.35 and w/c 0.3). These samples were cast in small plastic cylindrical molds of 30 mm X 50 mm size and kept sealed in airtight condition for 1 year.
Table 3.1: Bogue Composition of a typical Type I/II Portland cement.
Compound1 Short Form Weight (%) Alite or tricalcium silicate C3S 61
Belite or dicalcium silicate C2S 16
Tricalcium aluminate C3A 10
Tetracalcium aluminoferrite C4AF 8
Gypsum CSH2 6
Figure 3.1: Disk shaped and cylindrical cement samples of a) 0.42 b) 0.35 and c) 0.30 water to cement ratio.
Belite is impure dicalcium silicate (C2S) which along with alite (C3S) is responsible for
formation of calcium silicate hydrate (C-S-H) in cement paste. The overall reaction of alite and belite can be described chemically (approximately) as:
C3S + 5.3 H → C1.7-S-H4 + 1.3 CH
C2S + 4.3 H → C1.7-S-H4+ 0.3 CH
Here, H is water (H2O) and CH is calcium hydroxide. As seen from the two equations, the
primary hydration product of belite is C-S-H with a small amount of CH. This small amount of CH makes belite suitable for standard Calcium to Silicon ratio calibration in Energy Dispersive Spectroscopy (EDS) analysis. Its use as a calibration standard is described in more
1 In cement chemistry, C=CaO, S=SiO
2, A= Al2O3, S= SO3, F = Fe2O3, H=H2O. The atomic elements without
oxides are expressed in a conventional manner.
31 detail in Section 3.4.2. However, due to the slow reaction rate and strength development nature of belite, it is not used as the primary silicate in cement production.
In this study, A sample paste containing belite and distilled water was prepared with a w/c ratio ~ 0.42 (Figure 3.2) for standard calibration in EDS analysis. The sample was cast in small plastic cylindrical molds of 30 mm X 50 mm size and was kept in sealed condition for 2 months before subsequent surface preparation.
Figure 3.2: Disk shaped belite paste sample after removing from mold.
3.3 Sample preparation
3.3.1 Surface preparation
Achieving flat sample surface is important to ensure good geometry of micropillars in milling. Also, use of the nanoindentation system for micro-compression requires a flat surface with negligible slope for making proper contact between the indenter tip and the pillar top. If the sample surface is not flat enough, the pillar top will not be flat either, increasing the possibility of partial contact and eccentric loading instead of pure compression.
32 of excess moisture) of the sample. The air drying helps to prevent rapid drying, and associated excessive cracking of the sample during vacuum application at SEM.
Figure 3.3: a) Large scale saw, and b) Buehler Isomet low speed saw used for cutting cement sample.
Special attention is required in reducing the surface roughness of the saw cut specimens, since local waviness on sample surface could also be considered as a slope. Moreover, scanning electron microscopy, particularly, backscattered electron and X-ray imaging requires highly polished surface with minimum surface roughness for examination of microstructural details. To ensure smooth and flat surface with adequate surface roughness, thin slices were polished for 40 - 45 min using a 1200-grit SiC pad (Figure 3.4) and cleaned with acetone to remove residue. During polishing, consistent pressure was applied on the samples to have consistency in polished surface. Polished samples were observed carefully with naked eye for a mirrorlike reflective surface, and then with optical microscope to ensure suitability of the sample for application of scanning electron microscopy. The optical microscope micrograph in Figure 3.5 shows the appearance of polished cement samples.
Figure 3.4: Saw cut thin cement sample on polisher machine.